In-Situ X-ray Diffraction Studies of Host−Guest Properties in Nanoporous Zinc-Triazolate-Based Framework Materials
Halder, Gregory J.; Park, Hyunsoo; Funk, Russell J.; Chapman, Karena W.; Engerer, Laura K.; Geiser, Urs; Schlueter, John A.; Crystal Growth & Design 9 (2009) 3609–; doi:10.1021/cg900349c

data_4509562
_publ_section_title
;
 In-Situ X-ray Diffraction Studies of Host&#x2212;Guest Properties in
 Nanoporous Zinc-Triazolate-Based Framework Materials
;
_journal_issue                   8
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              3609
_journal_paper_doi               10.1021/cg900349c
_journal_volume                  9
_journal_year                    2009
_chemical_formula_moiety         'C18 H26 N32 O8 Zn7, 2(C2 H6 O)'
_chemical_formula_sum            'C22 H38 N32 O10 Zn7'
_chemical_formula_weight         1368.43
_chemical_melting_point          Zn~7~(AmTAZ)~8~(CO~3~)~2~(OH)~2~.2(EtOH)
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 97.259(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   26.352(3)
_cell_length_b                   22.909(2)
_cell_length_c                   16.5408(15)
_cell_measurement_reflns_used    1909
_cell_measurement_temperature    298(2)
_cell_measurement_theta_max      26.974
_cell_measurement_theta_min      2.577
_cell_volume                     9905.6(17)
_computing_cell_refinement       'SMART (BrukerAXS, 1997)'
_computing_data_collection       'SMART (BrukerAXS, 1997)'
_computing_data_reduction        'SAINT+ (BrukerAXS, 1997)'
_computing_molecular_graphics    'XPMA/ZORTEP, Webalb Viewer Pro 3.7'
_computing_publication_material  XCIF
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.967
_diffrn_measured_fraction_theta_max 0.967
_diffrn_measurement_device_type  'Siemens SMART CCD'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0520
_diffrn_reflns_av_sigmaI/netI    0.0507
_diffrn_reflns_limit_h_max       33
_diffrn_reflns_limit_h_min       -33
_diffrn_reflns_limit_k_max       30
_diffrn_reflns_limit_k_min       -30
_diffrn_reflns_limit_l_max       22
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            47449
_diffrn_reflns_theta_full        28.28
_diffrn_reflns_theta_max         28.28
_diffrn_reflns_theta_min         1.18
_exptl_absorpt_coefficient_mu    3.412
_exptl_absorpt_correction_T_max  0.843
_exptl_absorpt_correction_T_min  0.702
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   'SADABS, Bruker 1995'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    1.835
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'fine rectangular rod'
_exptl_crystal_F_000             5472
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.538
_refine_diff_density_min         -2.078
_refine_diff_density_rms         0.222
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.066
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     591
_refine_ls_number_reflns         11888
_refine_ls_number_restraints     9
_refine_ls_restrained_S_all      1.086
_refine_ls_R_factor_all          0.0804
_refine_ls_R_factor_gt           0.0528
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0960P)^2^+62.2104P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1630
_refine_ls_wR_factor_ref         0.1790
_reflns_number_gt                8583
_reflns_number_total             11888
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg900349csup1.cif
_cod_data_source_block           2.2(EtOH)
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1891 2012-01-12 08:04:46Z andrius 
;
_cod_original_cell_volume        9905.8(16)
_cod_database_code               4509562